Javanese volcanic allophane adsorbent as heavy metal adsorber to improve the quality of drinking water in surakarta
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201348Javanese Volcanic Allophane Adsorbent as Heavy Metal Adsorberto Improve the Quality of Drinking Water in SurakartaPranoto1*Suranto2Kristian H. Sugiyarto3Ashadi41. Department of Chemistry, Science and Mathematics Faculty, Sebelas Maret University2. Department of Biology, Science and Mathematics Faculty, Sebelas Maret University3. Department of Chemistry Education, Yogyakarta State University4. Department of Chemistry Education, Education Faculty, Sebelas Maret University* E-mail of the corresponding author: firstname.lastname@example.orgAbstractThe present study is concern with the identification, characterization and activation of natural allophane as anadsorbent of heavy metal ions Cr, Fe, Cd, Cu, Pb and Mn. The purposes of this study were to identify andcharacterize the natural allophane of Javanese volcanoes (Papandayan, Arjuna and Wilis), and to determine theoptimum conditions of adsorption and adsorption isotherms that happened. The identification of natural allophanewas performed by using NaF, pH, FTIR, and XRD. The characterization of the acidity of allophane was analyzedby using ammonia adsorption. The activation was done in the NaOH solution of 1 N and 3 N, and in the soakingtime of 1, 3, and 5 hours. The adsorption was done according to batch method with the variations of contact time of30, 60, 90 and 120 minutes. The adsorption isotherms performed by using the variations of the amount of adsorbate.Atomic Absorption Spectroscopy (AAS) was used in the analysis to determine the concentration of heavy metalions in solution. The results show that the analysis of NaF, pH, FTIR and XRD indicate the presence of allophanein the volcanic samples. The optimum conditions of activation and adsorption of the metal ions of Cr and Cd are inthe activation of NaOH 3N for 3 hours within 120 minutes contact time, those of metal ions of Fe are in theactivation of NaOH 3N for 1 hour within 30 minutes contact time, those of the metal ions of Pb and Mn are in theactivation of NaOH 3N for 5 hours within 90 minutes contact time, and those of metal ions of Cu are in theactivation of NaOH 3N for 5 hours within 60 minutes contact time. The adsorption isotherms performed to allkinds of metals follow Freundlich equation which suggests that physical interactions occur. Thus, an activationwith NaOH can increase the acidity of allophane causing to improve adsorption capacity to the metals by about50-100%..Keywords: allophane, heavy metals, adsorption1. IntroductionOne type of pollutants that requires a lot of attention in environmental management is that of heavy metals. Thedisposal of waste contaminated by heavy metals into water sources (ground water or surface water) becomes amajor problem of pollution because of its toxic and nonbiodegradable characteristics. The types of heavy metalsthat are considered as having a high level of toxicity are Hg, Cd, Cu, Ag, Ni, Pb, As, Cr, Sn, Zn and Mn(Suprihatin and Indrasti, 2010).Some of the most significant techniques to remove heavy metals in liquid wastes are: chemical precipitation,filtration, ion exchange resin, and a membrane system. The main thing to think of with these technologies is thatnot all metals can be removed, the reagents are high and they require much energy and high operating costs(Esmaili, et al., 2003). Lately, adsorption has become an alternative method for dissolving metal ions from liquidwastes. It is also used to minimize costs, and thus, as a kind of extensive research using a low-cost adsorbenttypes of soil (Potgeiter, et al., 2005).Allophane was found to be very good for adsorption of some heavy metals (e.g. Clark & McBride, 1984; Denaixet al, 1999, Abd-Elfatah & Wada, 1981). Iyoda et al (2011) reported the adsorption of heavy metals (Cu, Cd, Pb,and V) by natural and synthetic allophanes. An Al-rich allophane has also been synthesized, and a portion of theorganic matter was extracted from the clay fraction, and their reactivities towards Cu2+ orZ n2+ were studied bypotentiometry (Latrill et al, 2003). The synthetic allophane was usually prepared due to Wada et al (1979).Allophane may be defined as an amorphous clay mineral and a promising material which is naturally available involcanic soils. The single unit of allophane consists of a hollow spherule with a diameter of ~5 nm, and possessperforations in the wall with a (HO)Al(OH2) structure and diameter of ~0.3 nm (Iyoda et al, 2011). Thus, itshould be widely available in the wild, as is located in the flat to mountainous areas with an altitude of 0-3000 mabove sea level and is formed under the influence of wet tropical climate such as Indonesia.
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201349The activators H2SO4 and NaOH have been applied to determine the effect on the allophane’s surface widthand acidity (Widjanarko, et al, 2003). When they are compared, the activation with NaOH produces a widerspecific surface area than that with H2SO4.In this research, the identification, characterization, and activation of natural allophane with NaOH were applied.It was then used as an adsorbent in the removal of heavy metals in water.2. Materials and Methods2.1 Materials and ToolsThe main materials used in this study were allophane taken from volcanic mountains in Java (Papandayan,Arjuna and Wilis), distilled water, NaOH, NaF, pH stick, HNO3, ammonia, Whatman filter paper 42, and themodel of solution of metals Fe, Mn , Cr, Cd, Cu, Pb 1000 ppm.The particular tools used were furnace, 200 mesh sieve, a set of Atomic Absorption Spectroscopy (AAS) BrandShimadzu Type AA-6650 F, a set of X-Ray Diffraction (XRD) Brand Shimadzu Type 600, a set of FourierTransform Infra Red (FT-IR) Brand Shimadzu Type FT-IR-8201 PC, TOA pH meter, and desiccator.2.2 Preparation of Activated Allophane, Physical Characterization and MeasurementsThe natural allophane was aerated and then crushed. The powder obtained was sieved, which was then soaked indistilled water, filtered, and dried at a temperature of 105 0C for about 4 hours. The final product of driedallophane powder was then identified and characterized by NaF, FT-IR, and XRD.After activation process with 1 N and 3 N of NaOH within the time variations of 1, 3 and 5 hours, the activatedallophane, was finally used to adsorb the heavy metals, Fe, Mn Cr, Cd, Cu, and Pb, to determine the adsorptionisotherms, as well as to characterize the acidity. The natural allophane, without activation, was also used toabsorb the metals for comparison.3. Result and DiscussionAn initial test of the presence of allophane on the andisol ground was done by means of NaF-pH test. The NaF testresults for each of the mountains are shown in Table 1. The pH of all samples being greater than 9.4 shouldfonfirm that it is due to the presence of allophane (Munir, 1996).Table 1. pH NaF of samplesSample pH NaFMount Papandayan 11,08Mount Arjuna 12,20Mount Wilis 11,733.1 Infrared of allophane sample:3.1.1 Analysis of FTIRAs shown in Fig. 1a, the IR spectra for all natural samples are similar one to another, and they are typical forallophane as compared to the IR spectrum of allophane recorded by Devnita, et al. (2005) and shown in Fig. 1b.The details of analysis are recorded in Table 2.Figure 1. a. FTIR spectra of natural samples; b. FTIR spectrum of allophane (Devnita, et al., 2005)(a)(b)
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201350Table 2. The comparison between the spectra of samples and the analysis by Devnita, et al. (2005)Functional groupsAllophane uptake (cm-1)Devnita(2005)Papandayan Arjuna WilisVibration –OH (Al-OH/Si-OH) 3455 3437 3421,72 3444,87Vibration AlOH/SiOH 1108; 973 960,55; 991,41 912,33;1039,63 912,33;1035,77The existence of Si-O bond 579; 485 428,2 443,63; 468,7 426,27;432,053.1.2 XRD of Natural AllophaneX-Ry powder diffraction for the three samples were recorded, and as shown in Fig. 2 they are similar each others.The details of particular d-spacings are confirmed with JCPDS for allophane as shown in Table 3.Figure 2. XRD spectra of SamplesTable 3. Typical d-spacings data of the three samples compared to that of JCPDSJCPDS (38-0449)d-spacing(Å)3,300 2,250 1,860 1,400 1,230Papandayan 3,305 2,249 1,861 1,400 1,230Wilis 3,305 2,249 1,861 1,400 1,230Arjuna 3,305 2,249 1,861 1,400 1,2303.2 Adsorption of the Activated AllophaneThe natural (without activation) and the activated allophanes were then applied to adsorption of the solutionscontaining metal ions of Fe, Cr, Cu, Cd, Pb, and Mn within 30, 60, 90, and 120 minutes contact time of adsorption.The number of the heavy metals adsorbed was analyzed by AAS. The results were collected in Table 4 (for Cr andFe), Table 5 (for Pb and Mn), and Table 6 (for Cd and Cu).0100020003000400050006000700080009000100000 50 100ArjunaWilisPapandayan
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201351Table 4. The percentage of metal ions uptake of Cr and FeSample Metal TreatmentThe percentage of absorption(%)30’ 60’ 90’ 120’MountPapandayanChromiumWithoutactivation0 0.8 0 01N 1hour 51.8 55.8 63.5 60.91N 3 hours 51.7 65.0 70.2 71.41N 5 hours 70.0 74.1 80.1 76.03N 1 hour 76.7 89.8 88.0 86.83N 3 hours 82.9 95.7 97.6 97.83N 5 hours 64.2 75.8 65.1 93.2IronWithoutactivation96.3 94.7 94.0 86.41N 1 hour 97.5 96.9 95.8 95.31N 3 hours 98.1 96.8 93.9 88.91N 5 hours 97.9 95.8 95.4 95.23N 1 hour 99.9 98.7 94.5 93.23N 3 hours 99.7 96.8 96.3 95.93N 5 hours 97.2 95.9 95.8 86.8The adsorption performed on the initial concentration of 1 ppm and 5 ppm of metals Cr and Fe respectivelyproduced the adsorbents weighing 0.25 g and 0.5 g respectively. Table 4 shows that the optimum condition formetal adsorption of Cr-ions is on the activation with NaOH (3N) for 3 hours within 120 minutes contact time,while that of Fe-ions is on the activation of NaOH (3N) for 1 hour within 30 minutes contact time. Thepercentages of the maximum adsorptions of Cr and Fe metals to the activated allophane are 97% and 99.9%respectively. While for the iron adsorption there is not so significant allophane increased from 96.3 (withoutactivation) to about 100% (for the activated), it is significantly to be the case for Cr, being increased about 97%(for the activated) from none (without activation).Table 5. The percentage of metal ions uptake of Pb and MnSample Metal TreatmentThe percentage of absorption(%)30’ 60’ 90’ 120’Mount WilisLeadWithoutactivation13.1 12.0 15.9 14.91N 1hour 8.34 8.94 10.1 9.031N 3 hours 8.74 8.79 10.6 9.301N 5 hours 9.93 10.3 12.7 10.93N 1 hour 12.9 14.8 15.6 14.13N 3 hours 16.1 18.3 22.8 20.33N 5 hours 41.6 44.8 46.9 39.9ManganeseWithoutactivation42.9 12.2 9.21 16.91N 1 hour 12.9 25.6 7.36 33.91N 3 hours 41.2 29.3 26.8 11.71N 5 hours 50.2 38.6 34.6 24.63N 1 hour 50.5 48.5 49.7 43.13N 3 hours 79.5 77.2 74.2 71.83N 5 hours 82.8 86.8 88.8 79.7The adsorption performed on the initial concentrations of 40 ppm and 3 ppm of metals Pb and Mn respectivelyproduced the adsorbents weighing 0.25 g and 0.5 g respectively. Table 5 shows that the optimum condition formetal adsorption of Pb and Mn is on the activation with NaOH (3 N) for 5 hours within 90 minutes contact time.The percentages of the maximum adsorption of Pb and Mn metals to the activated allophane were found to be
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201352about 46.9% and 88.8% respectively. Thus, there is an increasing adsorption of Pb for about nearly three timesfrom 15.9% (without activation) to 46.9% (for the activated). The increasing adsorption of Mn was also observedin more significance; it is about nine times from only 9.21% (without activation) to 88.8% (for the activated).Table 6. The percentage of metal ions uptake of Cd and CuSample Metal TreatmentThe percentage of absorption(%)30’ 60’ 90’ 120’Mount ArjunaCadmiumWithoutactivation5.27 5.47 5.74 5.211N 1hour 90.8 97.3 94.4 88.731N 3 hours 98.3 97.2 91.0 91.681N 5 hours 64.0 93.4 97.8 92.313N 1 hour 64.0 96.5 97.8 92.313N 3 hours 93.9 97.9 97.2 98.83N 5 hours 90.2 97.4 96.8 95.20CopperWithoutactivation31.8 30.6 34.2 31.621N 1 hour 73.9 60.7 72.8 64.821N 3 hours 69.8 53.0 76.6 68.411N 5 hours 66.2 53.8 76.6 76.753N 1 hour 67.6 62.7 68.7 66.223N 3 hours 74.6 68.1 78.5 69.543N 5 hours 70.6 87.4 86.3 85.48The adsorption performed on the initial concentrations of 2 ppm of Cd and 4 ppm of Cu produced the adsorbentsweighing 0.5 g. Table 6 shows that the optimum condition of adsorption of Cd were is on the activation of NaOH (3N) for 3 hours within 120 minutes contact time , while that of Cu is on the activation of NaOH (3N) for 5 hourswithin 60 minutes contact time. The percentages of the maximum adsorption of Cd and Cu metals to the activatedallophane were found to be about 98.8% and 87.4% respectively. Thus, there is an huge increasing adsorption ofCd for more than sixteen times from 5.21% (without activation) to 98.8% (for the activated). The increasingadsorption of Cu was also observed in a slightly lesser significance; it is nearly three times from only 30.6%(without activation) to 87.4% (for the activated).It is not surprising that the difference in optimum adsorption conditions for each sample is affected by thedifference in ability of the adsorbent to adsorb the adsorbate and by the difference in characteristics of theadsorbate to be absorbed.3.3 Determination of the Type of Adsorption IsothermsThe determination of adsorption isotherms aims to know the types of adsorption to occur. The type ofadsorption is performed only for the activated allophane at the optimum conditions. Linear regression test isperformed by using Langmuir and Freundlich equations (Slejko: 1985; Helfferich: 1962), and the results areshown in Fig. 3 - Fig. 8.
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201353Figure 3. The isothermic curves of adsorption of Fe within contact time of 30 minutes by allophane of MountPapandayan activated with NaOH (3 N) in 1 hoursFigure 4. The isothermic curves of adsorption of Cr within contact time of 120 minutes by allophane of MountPapandayan activated with NaOH (3 N) in 3 hoursFigure 5. The isothermic curves of adsorption of Mn within contact time of 90 minutes by allophane of MountWilis activated with NaOH (3 N) in 5 hoursy = -0.0006x + 0.5409R² = 0.63870.50.510.520.530.540.550.560 20 40 60Langmuir isotherm curvey = 1.026x + 0.245R² = 0.99900.511.522.50 1 2Freundlich isothermic curvey = -0.0006x + 0.5409R² = 0.63870.50.510.520.530.540.550.560 20 40 60C/QCLangmuir isotherm curvey = 1.026x + 0.245R² = 0.99900.511.522.50 1 2LogQLog CFreundlich isothermic curvey = 0,963x + 0,236R² = 0,99800.511.520 0.5 1 1.5LogQLog CFreundlich isothermic curvey = 0.002x + 0.600R² = 0.4540.580.60.620.640.660 10 20 30C/QCLangmuir isothermic curvey = -0,000x + 0,542, R² = 0,8570.520.5250.530.5350.540.5450 20 40C/QCLangmuir isothermic curvey = 1.0166x + 0.2541R² = 100.511.520 0.5 1 1.5 2LogQLog CFreundlich isothermic curve
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201354Figure 6. The isothermic curves of adsorption of Pb within contact time of 90 minutes by allophane of MountWilis activated with NaOH (3 N) in 5 hoursFigure 7. The isothermic curves of adsorption of Cd within contact time of 120 minutes by allophane of MountArjuna activated with NaOH (3 N) in 3 hoursFigure 8. The isothermic curves of adsorption of Cu within contact time of 60 minutes by allophane of MountArjuna activated with NaOH (3 N) in 5 hoursLangmuir isotherm fits for the adsorption of a single adsorbate onto a series of equivalent sites on the surface ofthe solid. It may indicate that the adsorption process occurs “chemically” in which each group of activeadsorbents will only absorb one adsorbate species (metal ion), so it is limited only to the formation of a singlelayer (Slejko: 1985; Helfferich: 1962). This is a specific adsorption. On the other hand, the Freundlich isothermis the most important multisite adsorption isotherm for rough surfaces of the (allophane) solid (Futomo, et.al:1996). It may describe that the the adsorption occurs physically. Metal ions will only stick to the surface ofallophane and is not chemically tightly bonded so that they will be easily separated.Figures 3 to 8 exhibit significantly that the data of adsorption of the metal ions by the allophanes followsreadily Freundlich isotherm equation as indicated by the values of R2fitting to the linearity of the lines. Thi is inline with the adsorption by natural as well as synthetic allophanes reported by Iyoda et al (2011). Therefore, itmight be interpreted that the interaction that occurs in the adsorption is likely only physically in nature.3.4 Acidity CharacterizationThe measurements of acidity was performed with alkaline ammonia adsorption method, and again, this isonly to the activated allophane at the optimum conditions and the non-activated for comparison. The results ofacidity measurement are recorded as shown in Table 6.y = 0,643x + 0,496, R² = 0,94000.511.520 1 2LogQLog CFreundlich isothermic curvey = 0,012x + 0,663, R² = 0,73500.511.520 20 40 60 80C/QCLangmuir isothermic curvey = 4,776x - 1,653, R² = 0,7060510150 1 2 3C/QCLangmuir isotermic curvey = 0.526x + 0.134R² = 0.75800.510 0.5 1 1.5LogQLog CFreundlich isotermic curvey = 0.786x + 0.257, R² = 0.98800.511.50 0.5 1 1.5logQLog CFreundlich isothermic curvey = 28,76x - 16,49, R² = 0,855051015- 0.50 1.00C/QCLangmuir isothermic curve
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201355Table 6. The Acidity of Volcanic AllophanesSample Treatment Acidity (mmol/g)Mount PapandayanWithout activation 1,7045 ± 0,08563N 1Hours 2,2355 ± 0,16703N 3 Hours 2,8240 ± 0,1660Mount WilisWithout activation 2,8823± 0,24953N 5 Hours 6,4117±0,0832Mount ArjunaWithout activation 1,2941 ± 0,08323N 3 Hours 1,3529 ± 0,08323N 5 Hours 1,5882 ± 0,0831From the data in Table 6, it suggests that the acidity of the activated allophanes be greater than that of thenon-activated natural allophanes. This is likely due to the fact that the activation process can get rid of theimpurities attached to the allophanes and then the acid sites become visible.4. ConclusionA series of volcanic soils of Mountain Papandayan, Mountain Wilis, and Mountain Arjuna were found tocontain natural allophanes with difference in acidity and in capacity for adsorbing the metal ions. Activation withNaOH solution of 3N (within 1- 5 hours) to the allopanes resulted in the optimum and significant increase ofadsorbing the metal ions in a various contact time of 30 to 120 minutes. It was found that the allophane ofPapandayan was to be typical for adsorbing the metal ions of Cr and Fe, while allophane of Wilis was for themetal ions of Pb and Mn, and that of Arjuna was for the metal ions of Cd and Cu. The type of adsorptionisotherm follows readily Freundlich equation, suggesting typically for the rough surfaces of the allophanes andlikely physical adsorption. Thus, the potential of allophanes in the adsorption of heavy metal ions (Cr, Fe, Pb,Mn, Cd, and Cu) which pose a serious threat to the environment and human health shall be investigated soonwith an eye on an economic and viable water treatment technology, and the result should be reportedimmedaiately.ReferencesAbd-Elfattah, A., Wada, K., 1981. Adsorption of lead, copper, zinc, cobalt, and cadnium by soils that differ incation-exchange materials. J. Soil Sci. 32, 271-283.C. Latrill E, L. Denaix & I. Lamy, 2003, Interaction of copper and zinc with allophane and organic matter in theB horizon of an Andosol. European Journal of Soil Science, June, 54, 357–364Clark, C.J., McBride, M.B., 1984. Chemisorption of Cu(II) and Co(II) on allophane and imogolite. Clays ClayMiner. 32, 300-310.Denaix, L., Lamy, I., Bottero, J.Y., 1999. Structure and affinity towards Cd2+, Cu2+, Pb2+of synthetic colloidalamorphous aluminosilicates and their precursors. Colloids and Surfaces A: Physicochem. Eng. Aspects. 158,315-325.Devnita. R, Yuniarti. A, dan Hudhaya. R, 2005, Penggunaan Metoda Selektive Disolution dan SpektroskopiInframerah dalam Menentukan Kadar Alofan Andisol, Fakultas Pertanian UNPADEsmaili, A., Nasseri., S., Mahvi, A., Atash-Dehghan, R., 2003, Adsorption of Lead and Zinc Ions from aqueoussolution by Volcanic Ash Soil, Mining and Environment III Conference, Available online :http://www.x-cd.com/sudbury03/prof41.htmlF. Helfferich, 1962, Ion-exchange, McGraw-Hill, New York.F. Iyoda, S. Hayashi, S. Arakawa, M. Okamoto, 2011, Nanostructure and Adsorption Behavior ofNatural/Synthetic Allophanes. PPS-27, 27th World Congress of the Polymer Processing Society, May 10-14,Marrakech, Morocco.F.L. Slejko, 1985, Adsorption Technology: A Step by Step Approach to Process Evaluation and Applications,Marcel Dekker, New York.Fumoto, T., Iwama, H. and Amano, Y., 1996, Japanese Journal of Soil Science and Plant Nutrition. December,Vol. 67(6) p. 648-654.Heraldy E, Pranoto, Prowida Dini, 2004. Studi karakterisasi dan aktivasi alofan alam serta aplikasinyasebagai adsorben logan Zn menggunakan metode kolom. Jurnal Alchemy Vol.3 No.1, Maret 2004, hal 32-42.Jurusan Kimia, F. MIPA Universitas Sebelas Maret Surakarta.Isoyama M, Wada SI, 2007, Effect of Reaction Time on Pb Removal from Allophanic Ash Soil by Acid
Journal of Environment and Earth Science www.iiste.orgISSN 2224-3216 (Paper) ISSN 2225-0948 (Online)Vol. 3, No.5, 201356Washing, Soils and Foundations. Soils and Foundations, Vol. 47, issue 3, p. 629-633.Munir, M., 1996, Tanah -Tanah Utama Indonesia, Pustaka Jaya, Jakarta.Potgeiter, J., Potgeiter-Vermaak, S., Kalibatonga, P., 2005, Heavy Metals Removal from Solution byPaligorskite Clay, Minerals Engineering. PWS Publishing Company, USASuprihatin and N.S. Indrasti, 2010, Penyisihan Logam Berat dari Limbah Cair Laboratorium dengan metodePresipitasi dan Adsorpsi, Makalah Sains, Vol. 14, No. 1:44-50, Departemen Teknologi Industri Pertanian,Fakultas Teknologi Pertanian, Institut Pertanian Bogor, Bogor 16680, Indonesia.Wada, K., 1989, Allophane and Imogolite, Ch.21, p.1051 – 1087, In J. B. Dixon and S. B. Weed (ed), Minerals inSoil Environments, 2thEditionWada, S.I., Eto, A. and Wada, K. 1979. Sodium And Chloride Sorption By Imogolite And Allophanes. Journal ofSoil Science, 30, 347–355Widjanarko, D.M, Pranoto, Christina Y, 2003. Jurnal Alchemy vol.2 No.2 September 2003, hal 19-29, JurusanKimia, F. MIPA Univeritas Sebelas Maret SurakartaPranoto. Author was born on Banjarmasin, 30 October 1954. Author achieved his bachelor degree of Chemistryeducation in State University of Yogyakarta, Indonesia 1981, then he got master degree of Chemistry inWollongong University, New South Wales, Australia 1990. The author has major field of EnvironmentalChemistry.Suranto. Author was born on Surakarta, 20 August 1957. Author achieved his bachelor degree of Biology inSebelas Maret University, Indonesia 1983, then he got master degree of Botany/Plant Protein in University ofTasmania, Hobart, Australia 1991. Then he got his Ph.D degree of Botany/Molecular Plant Virology in LaTrobeUniversity, Melbourne, Australia 1998. The author has major field of Botany/Molecular Plant Virology. Theauthor is a ProfessorKristian H. SugiyartoAuthor was born on Surakarta, 15 September 1948. He achieved his bachelor degree of Chemistry Education inInstitute of Education Yogyakarta, Indonesia 1978, then his M. Sc. and Ph. D. degrees both in InorganicChemistry from The School of Chemistry, The University of New South Wales, Australia, in 1987 and 1993respectively. He is a Professor with major field of Coordination Chemistry.Ashadi. Author was born on Boyolali, 02 January 1951. Author achieved his bachelor degree of ChemistryEducation in Institute of Education Yogyakarta, Indonesia 1981, Then he got his Ph.D degree of Chemistry inInstitute of Education Jakarta, Indonesia 1990. The author has major field of Chemistry Education. The author isa Professor